Slow relaxation of magnetization in unprecedented Cu‒Ln-Rad hetero-tri-spin chains constructed from multidentate nitronyl nitroxide
Sun, Juan; Sun, Zan; Wang, Kang; Xi, Lu; Ma, Yue; Li, Licun; Journal of Materials Chemistry C 7 (2019) 9057–; doi:10.1039/C9TC02410G

data_7237868
_publ_section_title
;
 Slow relaxation of magnetization in unprecedented Cu--Ln-Rad
 hetero-tri-spin chains constructed from multidentate nitronyl nitroxide
;
_journal_issue                   29
_journal_name_full               'Journal of Materials Chemistry C'
_journal_page_first              9057
_journal_paper_doi               10.1039/C9TC02410G
_journal_volume                  7
_journal_year                    2019
_chemical_formula_sum            'C58 H32 Cu2 Dy F42 N4 O17'
_chemical_formula_weight         2144.48
_space_group_crystal_system      triclinic
_space_group_IT_number           2
_space_group_name_Hall           '-P 1'
_space_group_name_H-M_alt        'P -1'
_atom_sites_solution_hydrogens   mixed
_audit_creation_method           SHELXL-2014/7
_audit_update_record
;
2019-04-01 deposited with the CCDC.	2019-06-27 downloaded from the CCDC.
;
_cell_angle_alpha                74.60(3)
_cell_angle_beta                 85.46(3)
_cell_angle_gamma                87.18(3)
_cell_formula_units_Z            2
_cell_length_a                   12.222(2)
_cell_length_b                   16.580(3)
_cell_length_c                   20.905(4)
_cell_measurement_reflns_used    8157
_cell_measurement_temperature    113.1500
_cell_measurement_theta_max      27.8267
_cell_measurement_theta_min      1.4041
_cell_volume                     4069.5(14)
_computing_cell_refinement
;
CrystalClear-SM Expert 2.1 b42 (Rigaku, 2015)
;
_computing_data_collection
;
'CrystalClear-SM Expert 2.1 b42 (Rigaku, 2015)'
;
_computing_data_reduction
;
CrystalClear-SM Expert 2.1 b42 (Rigaku, 2015)
;
_computing_molecular_graphics    Diamond
_computing_publication_material  Diamond
_computing_structure_refinement  'SHELXL-2014/7 (Sheldrick, 2014)'
_computing_structure_solution    SHELXL
_diffrn_ambient_temperature      113.1500
_diffrn_measured_fraction_theta_full 0.998
_diffrn_measured_fraction_theta_max 0.998
_diffrn_measurement_device_type  'Rigaku Pilatus 200K'
_diffrn_measurement_method       'profile data from \w-scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0638
_diffrn_reflns_av_unetI/netI     0.0756
_diffrn_reflns_Laue_measured_fraction_full 0.998
_diffrn_reflns_Laue_measured_fraction_max 0.998
_diffrn_reflns_limit_h_max       14
_diffrn_reflns_limit_h_min       -14
_diffrn_reflns_limit_k_max       19
_diffrn_reflns_limit_k_min       -19
_diffrn_reflns_limit_l_max       24
_diffrn_reflns_limit_l_min       -24
_diffrn_reflns_number            39209
_diffrn_reflns_point_group_measured_fraction_full 0.998
_diffrn_reflns_point_group_measured_fraction_max 0.998
_diffrn_reflns_theta_full        25.009
_diffrn_reflns_theta_max         25.009
_diffrn_reflns_theta_min         1.274
_exptl_absorpt_coefficient_mu    1.584
_exptl_absorpt_correction_T_max  0.728
_exptl_absorpt_correction_T_min  0.628
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   SADABS
_exptl_crystal_colour            purple-green
_exptl_crystal_density_diffrn    1.750
_exptl_crystal_description       BLOCK
_exptl_crystal_F_000             2092
_exptl_crystal_size_max          0.3
_exptl_crystal_size_mid          0.25
_exptl_crystal_size_min          0.2
_refine_diff_density_max         2.050
_refine_diff_density_min         -1.530
_refine_diff_density_rms         0.146
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.000
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     1198
_refine_ls_number_reflns         14328
_refine_ls_number_restraints     119
_refine_ls_restrained_S_all      1.013
_refine_ls_R_factor_all          0.0934
_refine_ls_R_factor_gt           0.0762
_refine_ls_shift/su_max          0.004
_refine_ls_shift/su_mean         0.002
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.1272P)^2^+15.9686P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.2013
_refine_ls_wR_factor_ref         0.2175
_reflns_Friedel_coverage         0.000
_reflns_number_gt                11395
_reflns_number_total             14328
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            c9tc02410g2.cif
_cod_data_source_block           1_CCDC2
_cod_depositor_comments
;
The following automatic conversions were performed:

data item '_exptl_absorpt_correction_type' value 'Multi-scan' was
changed to 'multi-scan' in accordance with the
/home/saulius/struct/COD-crude-data/automatic-downloads/DataCite-retrospective/RSC/depositions/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 last updated on
2011-04-26.

Automatic conversion script
Id: cif_fix_values 6909 2019-04-08 15:41:33Z antanas 
;
_cod_database_code               7237868
_shelx_shelxl_version_number     2014/7
_shelx_res_checksum              61021
_shelx_fab_checksum              67455